Presentation on theme: "1 1 The Science and Engineering of Materials, 4 th ed Donald R. Askeland – Pradeep P. Phulé Chapter 15 - Polymers."— Presentation transcript:
1 1 The Science and Engineering of Materials, 4 th ed Donald R. Askeland – Pradeep P. Phulé Chapter 15 - Polymers
2 2 Objectives of Chapter 15 Discuss the classification of Polymers Learn two main ways of creating a Polymer Study the effect of temperature on Thermoplastics Study mechanical properties of Thermoplastics
3 3 Chapter Outline 15.1 Classification of Polymers 15.2 Addition Polymerization 15.3 Condensation Polymerization 15.4 Degree of Polymerization 15.5 Typical Thermoplastics 15.6 Structure–Property Relationships in Thermoplastics 15.7 Effect of Temperature on Thermoplastics
5 5 Section 15.1 Classification of Polymers Linear polymer - Any polymer in which molecules are in the form of spaghetti-like chains. Thermoplastics - Linear or branched polymers in which chains of molecules are not interconnected to one another. Thermosetting polymers - Polymers that are heavily cross-linked to produce a strong three dimensional network structure. Elastomers - These are polymers (thermoplastics or lightly cross-linked thermosets) that have an elastic deformation > 200%.
11 Example 15.1 Design/Materials Selection for Polymer Components Design the type of polymer material you might select for the following applications: a surgeon’s glove, a beverage container and a pulley. Example 15.1 SOLUTION The glove must be capable of stretching a great deal in order to slip onto the surgeon’s hand. This requirement describes an elastomer. A thermoplastic such as polyethylene terephthalate (PET) will have the necessary formability and ductility needed for this application. A relatively strong, rigid, hard material is required to prevent wear, so a thermosetting polymer might be most appropriate.
12 Section 15.2 Addition Polymerization Addition polymerization - Process by which polymer chains are built up by adding monomers together without creating a byproduct. Unsaturated bond - The double- or even triple- covalent bond joining two atoms together in an organic molecule. Functionality - The number of sites on a monomer at which polymerization can occur.
16 Example 15.2 Calculation of Initiator Required Calculate the amount of benzoyl peroxide initiator required to produce 1 kg of polyethylene with an average molecular weight of 200,000 g/mol. What is the degree of polymerization? Assume that 20% of the initiator is actually effective and that all termination occurs by the combination mechanism. Example 15.2 SOLUTION The molecular weight of ethylene = (2 C)(12) + (4 H)(1) = 28 g/mol. Therefore, the degree of polymerization is:
17 Example 15.2 SOLUTION (Continued) The combination mechanism requires the number of benzoyl peroxide molecules to be: The molecular weight of benzoyl peroxide is (14 C)(12) + (10 H)(1) + (4 O)(16) = 242 g/mol. Therefore, the amount of initiator needed to form the ends of the chains is:
18 Section 15.3 Condensation Polymerization Condensation polymerization - A polymerization mechanism in which a small molecule (e.g., water, methanol, etc.) is condensed out as a byproduct.
20 Example 15.3 Condensation Polymerization of 6,6-Nylon Nylon was first reported by Wallace Hume Carothers, of du Pont in about 1934. In 1939, du Pont’s Charles Stine reported the discovery of this first synthetic fiber to a group of 3000 women gathered for the New York World’s Fair. The first application was nylon stockings that were strong. Today nylon is used in hundreds of applications. Prior to nylon, Carothers had discovered neoprene (an elastomer). The linear polymer 6,6-nylon is to be produced by combining 1000 g of hexamethylene diamine with adipic acid. A condensation reaction then produces the polymer. Show how this reaction occurs and determine the byproduct that forms. How many grams of adipic acid are needed, and how much 6,6- nylon is produced, assuming 100% efficiency?
22 Example 15.3 SOLUTION (Continued) Molecular weight of hexamethylene diamine is 116 g/mol, of adipic acid is 146 g/mol, and of water is 18 g/mol. The number of moles of hexamethylene diamine added (calculated below) is equal to the number of moles of adipic acid: x = 1259 g of adipic acid required The number of moles of water lost is also 8.621: y = (8.621 moles) (18 g/mol) = 155.2 g H 2 O Total amount of nylon produced is 1000 g + 1259 g – 2(155.2 g) = 1948.6 g.
23 Section 15.4 Degree of Polymerization Degree of polymerization - The average molecular weight of the polymer divided by the molecular weight of the monomer.
25 Example 15.4 SOLUTION (Continued) The molecular weight of the repeat unit is the sum of the molecular weights of the monomers, minus that of the two water molecules that are evolved: M repeat unit = 116 + 146 – 2(18) = 226 g/mol Degree of polymerization = 120,000/226 = 531 The degree of polymerization refers to the total number of repeat units in the chain. The chain contains 531 hexamethylene diamine and 531 adipic acid molecules.
26 Example 15.5 Number and Weight Average Molecular Weights We have a polyethylene sample containing 4000 chains with molecular weights between 0 and 5000 g/mol, 8000 chains with molecular weights between 5000 and 10,000 g/mol, 7000 chains with molecular weights between 10,000 and 15,000 g/mol, and 2000 chains with molecular weights between 15,000 and 20,000 g/mol. Determine both the number and weight average molecular weights. Example 15.5 SOLUTION First we need to determine the number fraction x i and weight fraction f i for each of the four ranges. We can then use Equations 15-2 and 15-3 to find the molecular weights.
34 Section 15.6 Structure–Property Relationships in Thermoplastics Branched polymer - Any polymer consisting of chains that consist of a main chain and secondary chains that branch off from the main chain. Crystallinity is important in polymers since it affects mechanical and optical properties. Tacticity - Describes the location in the polymer chain of atoms or atom groups in nonsymmetrical monomers. Liquid-crystalline polymers - Exceptionally stiff polymer chains that act as rigid rods, even above their melting point.
39 Section 15.7 Effect of Temperature on Thermoplastics Degradation temperature - The temperature above which a polymer burns, chars, or decomposes. Glass temperature - The temperature range below which the amorphous polymer assumes a rigid glassy structure.
45 Figure 15.16 Photograph of spherulitic crystals in an amorphous matrix of nylon ( 200). (From R. Brick, A. Pense and R. Gordon, Structure and Properties of Engineering Materials, 4th Ed., McGraw-Hill, 1977.)
47 Example 15.6 Design of a Polymer Insulation Material A storage tank for liquid hydrogen will be made of metal, but we wish to coat the metal with a 3-mm thickness of a polymer as an intermediate layer between the metal and additional insulation layers. The temperature of the intermediate layer may drop to 80 o C. Design a material for this layer. Example 15.6 SOLUTION A material that has good ductility and/or can undergo large elastic strains is needed. We therefore would prefer either a thermoplastic that has a glass temperature below 80 o C or an elastomer, also with a glass temperature below 80 o C. Of the polymers listed in Table 15-2, thermoplastics such as polyethylene and acetal are satisfactory. Suitable elastomers include silicone and polybutadiene.
49 Example 15.7 Impact-Resistant Polyethylene A new grade of flexible, impact-resistant polyethylene for use as a thin film requires a density of 0.88 to 0.915 g/cm 3. Design the polyethylene required to produce these properties. The density of amorphous polyethylene is about 0.87 g/cm 3.
51 Example 15.7 SOLUTION We can use the data in Table 15-3 to calculate this density if we recognize that there are two polyethylene repeat units in each unit cell (see Example 3.16):
52 Example 15.7 SOLUTION (Continued) We know that ρ a = 0.87 g/cm 3 and that ρ varies from 0.88 to 0.915 g/cm 3. The required crystallinity then varies from: Therefore, we must be able to process the polyethylene to produce a range of crystallinity between 9.2 and 39.6%.
53 Section 15.8 Mechanical Properties of Thermoplastics Viscoelasticity - The deformation of a material by elastic deformation and viscous flow of the material when stress is applied. Relaxation time - A property of a polymer that is related to the rate at which stress relaxation occurs.
56 Example 15.8 Comparing Mechanical Properties of Thermoplastics Compare the mechanical properties of LD polyethylene, HD polyethylene, polyvinyl chloride, polypropylene, and polystyrene, and explain their differences in terms of their structures. Example 15.8 SOLUTION Let us look at the maximum tensile strength and modulus of elasticity for each polymer.
57 Example 15.8 SOLUTION (Continued) We can conclude that: 1. Branching, which reduces the density and close packing of chains, reduces the mechanical properties of polyethylene. 2. Adding atoms or atom groups other than hydrogen to the chain increases strength and stiffness. The methyl group in polypropylene provides some improvement, the benzene ring of styrene provides higher properties, and the chlorine atom in polyvinyl chloride provides a large increase in properties.
60 Example 15.9 Design of Initial Stress in a Polymer A band of polyisoprene is to hold together a bundle of steel rods for up to one year. If the stress on the band is less than 1500 psi, the band will not hold the rods tightly. Design the initial stress that must be applied to a polyisoprene band when it is slipped over the steel. A series of tests showed that an initial stress of 1000 psi decreased to 980 psi after six weeks. Example 15.9 SOLUTION We can use Equation 15-5 and our initial tests to determine the relaxation time for the polymer:
61 Example 15.9 SOLUTION (Continued) Now that we know the relaxation time, we can determine the stress that must be initially placed onto the band in order that it still be stressed to 1500 psi after 1 year (52 weeks). The polyisoprene band must be made significantly undersized so it can slip over the materials it is holding together with a tension of 1788 psi. After one year, the stress will still be 1500 psi.
63 Section 15.9 Elastomers (Rubbers) Geometric isomer - A molecule that has the same composition as, but a structure different from, a second molecule. Diene - A group of monomers that contain two double- covalent bonds. These monomers are often used in producing elastomers. Cross-linking - Attaching chains of polymers together to produce a three-dimensional network polymer. Vulcanization - Cross-linking elastomer chains by introducing sulfur or other chemicals.
83 Example 15.10 Insulation Boards for Houses You want to design a material that can be used for making insulation boards that are approximately 4 ft wide and 8 ft tall. The material must provide good thermal insulation. What material would you choose? Example 15.10 SOLUTION Glasses tend to be good insulators of heat. However, they will be heavy, more expensive, and prone to fracture. Polymers are lightweight, can be produced inexpensively, and they can be good thermal insulators. We can use foamed polystyrene since the air contained in the pores adds significantly to their effectiveness as thermal insulators. Finally, from a safety viewpoint, we want to be sure that some fire and flame retardants are added to the foams. Such panels are made using expanded polystyrene beads containing pentane.